Effects of Surface Treatments and Cement Types on the Bond Strength of Porcelain-to-Porcelain Repair Fatma Faiez Mohamed, BDS, MS,1 Matthew Finkelman, PhD,2 Roya Zandparsa, DDS, MSc, DMD,3 Hiroshi Hirayama, DDS, DMD, MS,3 & Gerard Kugel, DMD, MS, PhD3 1
Department of Oral Health Sciences, School of Dentistry, University of Michigan, Ann Arbor, MI Department of Public Health and Community Service, Tufts University School of Dental Medicine, Boston, MA 3 Department of Prosthodontics and Operative Dentistry, Tufts University School of Dental Medicine, Boston, MA 2
Keywords Shear bond strength; ceramic failure; composite/porcelain repair; silane coupling agent; surface treatments. Correspondence Fatma Mohamed, University of Michigan – Oral Health Sciences, 1011 N. University, Ann Arbor, MI 48109. E-mail: [email protected]
The authors deny any conflicts of interest. Accepted March 7, 2014 doi: 10.1111/jopr.12194
Abstract Purpose: The purpose of this in vitro study was to evaluate the effects of four surface treatments and two resin cements on the repair bond strength of a ceramic primer. Materials and Methods: Eighty-eight pairs of disks (10 and 5 mm in diameter, 3 mm thickness) were prepared from heat-pressed feldspar ceramics (GC Initial IQ). After being stored in mucin-artificial saliva for 2 weeks, the 10-mm disks were divided into four surface treatment groups (n = 22) and then treated as follows: (1) no treatment (control); (2) 40% phosphoric acid; (3) 5% hydrofluoric acid + acid neutralizer + 40% phosphoric acid; (4) silica coating (CoJet-sand) + 40% phosphoric acid. The 5-mm disks were treated with 5% hydrofluoric acid + 40% phosphoric acid. The two sizes of porcelain disks, excluding the control group, were primed with Clearfil Ceramic Primer. The specimens in each group were further divided into two subgroups of 11 each, and bonded with Clearfil Esthetic Cement (CEC) or Panavia F 2.0 Cement (PFC). The specimens were stored in distilled water at 37°C for 24 hours, thermocycled for 3000 cycles at 5 to 55°C, and stored at 37°C for an additional 7 days. Shear bond strength (SBS) was measured with a universal testing machine at a 0.5 mm/min crosshead speed until fracture. Statistical analysis of the results was carried out with a two-way ANOVA and Tukey HSD test (α = 0.05). Debonded specimen surfaces were examined under an optical microscope to determine the mode of failure. Results: The statistical analysis showed that the SBS was significantly affected by surface treatment and resin cement (p < 0.05). For treatment groups bonded with CEC, the SBS (MPa) values were (1) 2.64 ± 1.1, (2) 13.31 ± 3.6, (3) 18.88 ± 2.6, (4) 14.27 ± 2.7, while for treatment groups cemented with PFC, the SBS (MPa) values were (1) 3.04 ± 1.1, (2) 16.44 ± 3.3, (3) 20.52 ± 2.2, and (4) 16.24 ± 2.9. All control specimens exhibited adhesive failures, while mixed types of failures were observed in phosphoric acid-treated groups. The other groups revealed mainly cohesive and mixed failures. Conclusions: Combined surface treatment of etching with hydrofluoric acid and phosphoric acid provides the highest bond strengths to porcelain. Also, PFC exhibited higher SBS than CEC did.
Metal ceramic restorations have been widely used in dentistry for several decades1,2 due to their predictable strength and performance.3 However, failure of these restorations may occur when the veneering porcelain fractures,4-7 compromising esthetics and function.6 Previous clinical studies on metal ceramic crowns and partial fixed dental prostheses reported that fractures of veneering porcelain occur 2.38% to 8% of the time.8,9 This rate may increase even more with implantsupported metal ceramic restorations.10 Replacement of a failed
restoration, without compromising the supporting structure, is difficult, and is not practical, considering replacement cost and time.7,11-13 Various clinical techniques, direct and indirect, for repairing metal ceramic restorations have been described,9,14-17 offering less expensive and conservative alternatives to direct replacement.9 The success of the repair is largely dependent on the strength and durability of the bond between a repair material and porcelain. Various surface treatments, which either mechanically
C 2014 by the American College of Prosthodontists Journal of Prosthodontics 00 (2014) 1–8
Bond Strengths of Porcelain-to-Porcelain Repair
Mohamed et al
or chemically enhance bond strength, have been proposed. Mechanical bonding can be promoted by treatments such as acid etching with hydrofluoric acid (HF),11,18,19 phosphoric acid,20,21 or with acidulated phosphate fluoride;22,23 airborneparticle abrasion with aluminum oxide1,24 or silica-coated alumina particles;2,6,25,26 or roughening with a diamond rotary instrument.20 In addition, chemical bonding can be achieved by a silane coupling agent.13,19,27-29 Finally, an application of a layer of glass fiber-reinforced composite resin on the surface under the repair composite resin has also been suggested.30 However, it remains uncertain as to which procedure provides the best clinical results. Etching silica-based ceramics (i.e., feldspathic porcelain) with HF creates micromechanical undercuts on the surface. HF selectively dissolves the glass matrix of porcelain and exposes the crystalline structure,12,31 so the repair material can penetrate the undercuts and form micromechanical interlocking with the resin composite.32 However, HF is known to have hazardous effects on human tissue,31 and concerns about its use intraorally have been reported.1,23 To protect adjacent teeth and tissue, using a rubber dam and sodium bicarbonate/calcium source acid neutralizing medium is recommended.12 A chairside silica-coating technique that involves airborne particle abrasion with silica-modified Al2 O3 particles has also been described for repair of fractured metal ceramic restorations.33 Silica-coating treatment provides ultrafine mechanical retention, as well as chemical adhesion between the composite resin and the ceramic or metal, using the silane coupling agent.5,26 Ozcan and Niedermeier5 showed that intraoral silica coating of 289 fractured metal ceramic restorations, using the CoJet system, resulted in an 89% success rate after 3 years. Composite resins used in repair have also been shown to affect bond strength.29,34 It has been reported that large particlesize composites or hybrid type resins at the porcelain interface result in higher bond strengths than small particle-size composites,35 and that resin cement containing filler demonstrates better mechanical properties than resin cement without fillers.36 Matsumura et al37 reported that dual-cure cement exhibited greater bond strength than chemically activated cement, but also stated that this difference could be due to the presence of an adhesive monomer (MDP) in only one of the two cements, rather than the mode of activation. MDP is a dual-functional phosphate monomer, referring to 10-methacryloyloxydecyl dihydrogen phosphate monomer. The effect of resin cements on bond strength, depending on the absence or presence of MDP, is less certain. With the introduction of silanes in the early 1960s,38 chemical adhesion between resin composite and porcelain could be achieved. The silane coupling agent γ -methacryloxypropyl trimethoxysilane is a bi-functional molecule consisting of a silanol group that reacts with (-OH) groups on the porcelain surface, and a methacrylate group that copolymerizes with the resin matrix of the composite, forming siloxane bonds. It also enhances the resin bond by improving wettability of the ceramic surface.28 The silane coupling agent, which is included in several repair systems, showed enhanced repair bond strength of porcelain.12,19,27,29 Many efforts have been made to improve the effectiveness of silanes by using either heat treatment, through 2
warm-air drying,28 carbon dioxide laser irradiation,39 or by acid catalysis.28 Some silane coupling agents were effective after acid etching with phosphoric acid.36,40 A single-step silane primer, Clearfil Ceramic Primer (Kuraray Medical, Okayama, Japan), indicated for ceramic repair, has been developed. There is little information concerning its bond strength to porcelain. This primer contains the silane coupling agent and the adhesive monomer MDP in ethanol solvent. The aim of this in vitro study was to evaluate effects of four surface treatments and two dual-cure resin cements on the repair bond strength of the silane primer to porcelain.
Materials and methods Information on the materials used in this study is summarized in Table 1. Feldspathic porcelain (GC Initial IQ – One-Body, Press-over-Metal) indicated for metal ceramic restorations was used as a substrate material. Eighty-eight pairs of porcelain disks were fabricated using a heat-pressing technique. Two sizes of porcelain disks were made from wax patterns approximately 10 and 5 mm in diameter (3.5 mm thickness). The patterns were sprued, invested, and heat pressed according to the manufacturer’s instructions. Following the heat-pressing procedure, investment disks were bench cooled and divested by airborne-particle abrasion with 50-μm aluminum oxide at 2-bar pressure, and the attached sprue was carefully cut. Surface preparation of 10-mm diameter disks
To simulate exposure to the oral environment after porcelain fracture, the 10-mm disks were stored in artificial saliva (Mouth Kote; Parnell Pharmaceuticals, Inc., San Rafael, CA) for 2 weeks. Next, each disk was inserted in a ring with poly(methyl methacrylate) resin (Dentsply Caulk, Milford, DE), ensuring that the bonding surface was left uncovered. Then, each disk’s bonding surface was roughened sequentially under running water with 240-, 320-, and 600-grit abrasive papers (Buehler, Ltd., Lake Bluff, IL). No ultrasonic cleaning was done because this would be clinically impossible during an intraoral repair. The disks were divided equally into four groups (n = 22), each receiving one of the four treatments as follows: Group 1: No further treatment after grinding with abrasive papers (Control). Group 2: Etching with 40% phosphoric acid gel (K-Etchant; Kuraray Medical, Inc.) for 5 seconds, then washed, and dried. Group 3: Etching with